<p>Yes, some infill patterns are better than others for preventing separation of layers. Basically (modulo some assumptions about uniformity of distribution of force), the shearing strength of the part in the Z direction at a particular layer is going to be proportional to the <em>surface area</em> of bonding between successive layers. So infill patterns that stack identical infill extrusions on top of each other at each layer should be expected to be much stronger than patterns where successive layers make only partial contact. In other words, "2D infill patterns" - grid, lines, triangles, tri-hexagon - should be a lot stronger than "3D infill patterns" - cubic, octet, gyroid, ... This matches my experience printing bolts oriented along the Z-axis - ones printed with gyroid snap easily unless other measures are taken to strengthen them, while ones printed with triangles are fairly strong (though nowhere near as strong as ones printed oriented in the XY plane.</p>

<p>If you have other reason to prefer a "3D infill pattern", its weakness can be mitigated mostly by increasing the infill line width, so that the lines of successive layers which don't entirely overlap still touch on more surface area. (Just increasing the infill line width also works to make "2D infill patterns" even stronger.) However, be aware that with high print speed typically used for infill, increasing infill line width can easily exceed the capability of your hotend, resulting in underextrusion, extruder skipping, and stringing all over the place.</p>

CC BY-SA 4.0
2020-02-11T21:24:57.427Z
The main point of what I was saying is if you can change the orientation of your print so the stress is through the X or Y planes instead of the Z plane, the part will be much stronger. If strength is a factor and you're going to load the part, print orientation really needs to be looked at. I take your point about more surface area is going to be better. For that matter, 100% infill is going to work best, then, however, it still won't be as strong as what you'd find in the X/Y direction.
Pᴀᴜʟsᴛᴇʀ2
CC BY-SA 4.0
2020-02-11T21:43:22.593Z
@Pᴀᴜʟsᴛᴇʀ2: Indeed, that will help more, but if you have constraints that preclude changing the orientation or competing goals that would make it into a trade-off, choosing a different infill pattern can be part of the solution (often even a complete solution).
R.. GitHub STOP HELPING ICE
CC BY-SA 4.0
2020-02-11T20:24:44.293Z
2020-02-11T20:35:28.490Z
2020-02-11T20:35:28.490Z
R.. GitHub STOP HELPING ICE
<p>The shearing strength characteristics, or better known as interlaminar shear strength (ILSS) characteristics, describe the shear strength between the layers. This is also known as flexural or bending strength characteristics. These are best obtained by performing a 3- or 4-point bending test; these tests are standardized by the American Society for Testing and Materials, ASTM International (e.g. ASTM D 7264).</p>

<p>The bending test will cause internal compression (concave side during testing) and internal tension stresses (convex side during testing). The figure below shows the general setup of a 3-point bending test and below that  magnification of the stresses inside the test specimen.</p>

<p><a href="https://i.sstatic.net/GFMB5.png" rel="nofollow noreferrer"><img src="https://i.sstatic.net/GFMB5.png" alt="enter image description here"></a></p>

<p>The tests concern the interlaminar shearing of layers, so, the much more material a layer consists of (e.g. infill percentage) the higher the resistance against shearing off. Also, how the infill is internally supported by its form helps, if it buckles easily on the compression side, the buckling occurs before shear off. </p>

<p>Not only the type and percentage of infill is important for the flexural strength, but also the layer height, nozzle diameter print temperature as found in <a href="https://www.researchgate.net/publication/323878149_Strength_of_PLA_Components_Fabricated_with_Fused_Deposition_Technology_using_a_Desktop_3D_Printer_as_a_Function_of_Geometrical_Parameters_of_the_Process/link/5b9becf0299bf13e60316784/download" rel="nofollow noreferrer">this research paper</a>. Another paper, <a href="https://www.researchgate.net/publication/328848028_Effect_of_infill_on_tensile_and_flexural_strength_of_3D_printed_PLA_parts" rel="nofollow noreferrer">"Effect of infill on tensile and flexural strength of 3D printed PLA parts"</a> directly answers your question, quoting the figure from the paper:</p>

<p><a href="https://i.sstatic.net/euoYn.png" rel="nofollow noreferrer"><img src="https://i.sstatic.net/euoYn.png" alt="enter image description here"></a></p>

<p>You should choose an infill that has the most support. Since year and day, in creating composite sandwich panels (often used in aerospace applications where high stiffness and low weight are essential) <a href="https://en.wikipedia.org/wiki/Honeycomb_structure" rel="nofollow noreferrer">honeycomb core structures</a> are used as these honeycomb structures allow minimization of the amount of weight and used material. From the figure above you see that rectangular infill is best suited for FFF products. Honeycomb is the second best, but significantly lower. Note that orientation is key! E.g. <a href="https://www.cartesiancreations.com.au/gyroid-infill-tests/" rel="nofollow noreferrer">this test conducted by Martin</a> shows that Gyroid and honeycomb infill performs better than rectilinear:</p>

<p><a href="https://i.sstatic.net/OVdMG.png" rel="nofollow noreferrer"><img src="https://i.sstatic.net/OVdMG.png" alt="enter image description here"></a></p>

<p>To answer your question, not only infill pattern, but also infill density, nozzle diameter, layer height and orientation play an important role in the shearing strength. This is why ASTM has defined a standard so that we can compare results amongst different materials or different lay- or set-ups. These tests are typically performed dynamically (alternating load), statically with increasing load (increasing load with time) or statically fixed load (constant load to determine the creep properties, these test typically take a long time when the load is low).</p>

CC BY-SA 4.0
2020-02-13T13:42:59.883Z
The first paper (where you also took the graph from) does not mention anywhere the weight. Different infills produce often different final infill weight, as CNC kitchen (check on Youtube) found out. Unless the article explicitly states the issue and states that the infill percent had been corrected for it, we should not assume the procedure was correct. I guess they completely ignored the issue.
FarO
CC BY-SA 4.0
2020-02-13T13:56:29.057Z
@FarO Weight equals infill pattern and infill density, a wavy pattern creates more infill per mm product, so weight does not have to be explicitly mentioned. Please give a link for the CNC video, I cannot find any regarding shear strength characteristics.
0scar
CC BY-SA 4.0
2020-02-13T14:23:10.267Z
The effect I was mentioning: 10% infill results in different amount of material depending on the chosen infill pattern: https://youtu.be/upELI0HmzHc?t=206
FarO
CC BY-SA 4.0
2020-02-13T18:01:18.260Z
@FarO Exactly what I'm saying in answer and comments.
0scar
CC BY-SA 4.0
2020-02-12T06:49:59.083Z
2020-02-12T07:21:21.000Z
2020-02-12T07:21:21.000Z
0scar
<p>0scar's answer is the "solution" or true answer to the question.</p>

<p>Watching youtube the last few days, cubic needs to be considered. I was surprised at what I saw. More to consider is adding design elements:</p>

<ul>
<li>The concept of flutes along the perimeter.</li>
<li>Adding through holes increases strength incredibly.</li>
</ul>

CC BY-SA 4.0
2020-02-12T19:57:50.497Z
2020-02-12T19:57:50.497Z
Krista K
<p>For practicality sake, I need to print a design such that there will be weight hanging parellel to the layer lines. Is there an infill pattern that would be better than others at handling this?</p>

<p>I realize that all kinds of infill will still have the same layer boundaries. Just wondering if choosing any given infill might provide better results.</p>

CC BY-SA 4.0
2020-02-11T11:06:03.943Z
CNC-Kitchen anyone?
Trish
CC BY-SA 4.0
2020-02-11T12:48:45.337Z
If your layer lines are a concern for strength, different infill patters won't help because they are on the same layer lines (as you suggest). Your best bet is to reconfigure the print so the layer lines are no longer an issue, or consider creating the object using a different medium. Sometimes "practical" doesn't get the job done. If the part doesn't work, it doesn't make your life any easier :o)
Pᴀᴜʟsᴛᴇʀ2
CC BY-SA 4.0
2020-02-11T16:00:12.073Z
Wondering if it's possible to designate "spiralization" for infil independent of the structure's walls?   But I agree with paulster that you should consider reorienting the print so the layers are perpendicular to the hanging mass.  Alternatively, make the part into 2 or more pieces so as to achieve desired layer orientations.
Carl Witthoft
<fdm><infill><print-strength>
What is the best infill pattern for shearing strength?
linuxdan
# What is the best infill pattern for shearing strength?

(Asked by: username_0 on 2020-02-11)

For practicality sake, I need to print a design such that there will be weight hanging parellel to the layer lines. Is there an infill pattern that would be better than others at handling this?

I realize that all kinds of infill will still have the same layer boundaries. Just wondering if choosing any given infill might provide better results.

**Tags:** fdm, infill, print-strength
> **Comments:**
> **username_1**: CNC-Kitchen anyone?  
> **username_2**: If your layer lines are a concern for strength, different infill patters won't help because they are on the same layer lines (as you suggest). Your best bet is to reconfigure the print so the layer lines are no longer an issue, or consider creating the object using a different medium. Sometimes "practical" doesn't get the job done. If the part doesn't work, it doesn't make your life any easier :o)  
> **username_3**: Wondering if it's possible to designate "spiralization" for infil independent of the structure's walls?   But I agree with paulster that you should consider reorienting the print so the layers are perpendicular to the hanging mass.  Alternatively, make the part into 2 or more pieces so as to achieve desired layer orientations.  

---

## 3 answers

### Answer by username_4 on 2020-02-11. Score: 2

Yes, some infill patterns are better than others for preventing separation of layers. Basically (modulo some assumptions about uniformity of distribution of force), the shearing strength of the part in the Z direction at a particular layer is going to be proportional to the *surface area* of bonding between successive layers. So infill patterns that stack identical infill extrusions on top of each other at each layer should be expected to be much stronger than patterns where successive layers make only partial contact. In other words, "2D infill patterns" - grid, lines, triangles, tri-hexagon - should be a lot stronger than "3D infill patterns" - cubic, octet, gyroid, ... This matches my experience printing bolts oriented along the Z-axis - ones printed with gyroid snap easily unless other measures are taken to strengthen them, while ones printed with triangles are fairly strong (though nowhere near as strong as ones printed oriented in the XY plane.

If you have other reason to prefer a "3D infill pattern", its weakness can be mitigated mostly by increasing the infill line width, so that the lines of successive layers which don't entirely overlap still touch on more surface area. (Just increasing the infill line width also works to make "2D infill patterns" even stronger.) However, be aware that with high print speed typically used for infill, increasing infill line width can easily exceed the capability of your hotend, resulting in underextrusion, extruder skipping, and stringing all over the place.

> **Comments:**
> **username_2**: The main point of what I was saying is if you can change the orientation of your print so the stress is through the X or Y planes instead of the Z plane, the part will be much stronger. If strength is a factor and you're going to load the part, print orientation really needs to be looked at. I take your point about more surface area is going to be better. For that matter, 100% infill is going to work best, then, however, it still won't be as strong as what you'd find in the X/Y direction.  
> **username_4**: @Pᴀᴜʟsᴛᴇʀ2: Indeed, that will help more, but if you have constraints that preclude changing the orientation or competing goals that would make it into a trade-off, choosing a different infill pattern can be part of the solution (often even a complete solution).  

---

### Answer by username_5 on 2020-02-12. Score: 1

The shearing strength characteristics, or better known as interlaminar shear strength (ILSS) characteristics, describe the shear strength between the layers. This is also known as flexural or bending strength characteristics. These are best obtained by performing a 3- or 4-point bending test; these tests are standardized by the American Society for Testing and Materials, ASTM International (e.g. ASTM D 7264).

The bending test will cause internal compression (concave side during testing) and internal tension stresses (convex side during testing). The figure below shows the general setup of a 3-point bending test and below that magnification of the stresses inside the test specimen.

[![enter image description here](https://i.sstatic.net/GFMB5.png)](https://i.sstatic.net/GFMB5.png)

The tests concern the interlaminar shearing of layers, so, the much more material a layer consists of (e.g. infill percentage) the higher the resistance against shearing off. Also, how the infill is internally supported by its form helps, if it buckles easily on the compression side, the buckling occurs before shear off.

Not only the type and percentage of infill is important for the flexural strength, but also the layer height, nozzle diameter print temperature as found in [this research paper](https://www.researchgate.net/publication/323878149_Strength_of_PLA_Components_Fabricated_with_Fused_Deposition_Technology_using_a_Desktop_3D_Printer_as_a_Function_of_Geometrical_Parameters_of_the_Process/link/5b9becf0299bf13e60316784/download). Another paper, ["Effect of infill on tensile and flexural strength of 3D printed PLA parts"](https://www.researchgate.net/publication/328848028_Effect_of_infill_on_tensile_and_flexural_strength_of_3D_printed_PLA_parts) directly answers your question, quoting the figure from the paper:

[![enter image description here](https://i.sstatic.net/euoYn.png)](https://i.sstatic.net/euoYn.png)

You should choose an infill that has the most support. Since year and day, in creating composite sandwich panels (often used in aerospace applications where high stiffness and low weight are essential) [honeycomb core structures](https://en.wikipedia.org/wiki/Honeycomb_structure) are used as these honeycomb structures allow minimization of the amount of weight and used material. From the figure above you see that rectangular infill is best suited for FFF products. Honeycomb is the second best, but significantly lower. Note that orientation is key! E.g. [this test conducted by Martin](https://www.cartesiancreations.com.au/gyroid-infill-tests/) shows that Gyroid and honeycomb infill performs better than rectilinear:

[![enter image description here](https://i.sstatic.net/OVdMG.png)](https://i.sstatic.net/OVdMG.png)

To answer your question, not only infill pattern, but also infill density, nozzle diameter, layer height and orientation play an important role in the shearing strength. This is why ASTM has defined a standard so that we can compare results amongst different materials or different lay- or set-ups. These tests are typically performed dynamically (alternating load), statically with increasing load (increasing load with time) or statically fixed load (constant load to determine the creep properties, these test typically take a long time when the load is low).

> **Comments:**
> **username_6**: The first paper (where you also took the graph from) does not mention anywhere the weight. Different infills produce often different final infill weight, as CNC kitchen (check on Youtube) found out. Unless the article explicitly states the issue and states that the infill percent had been corrected for it, we should not assume the procedure was correct. I guess they completely ignored the issue.  
> **username_5**: @FarO Weight equals infill pattern and infill density, a wavy pattern creates more infill per mm product, so weight does not have to be explicitly mentioned. Please give a link for the CNC video, I cannot find any regarding shear strength characteristics.  
> **username_6**: The effect I was mentioning: 10% infill results in different amount of material depending on the chosen infill pattern: https://youtu.be/upELI0HmzHc?t=206  
> **username_5**: @FarO Exactly what I'm saying in answer and comments.  

---

### Answer by username_7 on 2020-02-12. Score: 0

0scar's answer is the "solution" or true answer to the question.

Watching youtube the last few days, cubic needs to be considered. I was surprised at what I saw. More to consider is adding design elements:

* The concept of flutes along the perimeter.
* Adding through holes increases strength incredibly.


---

